#------------------------------------------------------------------------------
#$Date: 2016-03-25 09:31:10 +0100 (vie 25 de mar de 2016) $
#$Revision: 179752 $
#$URL: svn://www.crystallography.net/cod/cif/7/00/48/7004821.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7004821
loop_
_publ_author_name
'León-Reina, L'
'Porras-Vázquez, J M'
'Losilla, E. R.'
'Sheptyakov, D. V.'
'Llobet, A.'
'Aranda, M. A. G.'
_publ_section_title
;
 Low temperature crystal structures of apatite oxygen-conductors
 containing interstitial oxygen.
;
_journal_issue                   20
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              2058
_journal_page_last               2064
_journal_year                    2007
_chemical_formula_sum            'Ge La1.44 O4.39 Sr0.23'
_chemical_formula_weight         362.78
_chemical_name_systematic        ' ?'
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            6
_cell_length_a                   9.8914(6)
_cell_length_b                   9.8914
_cell_length_c                   7.3184(5)
_cell_volume                     620.10(6)
_pd_block_id
2006-11-06T16:15|La865Sr135Ge_LT_phase1|M._A._G._Aranda||
_pd_phase_name
'from C:/RIETVELD/Apatito/SINQ_02/La9.55Si/La955Si6_RT/LA955SI.EXP'
_cod_data_source_file            1.cif
_cod_data_source_block           La865Sr135Ge_LT_phase_1
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (324
times).

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (103 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        620.10(10)
_cod_database_code               7004821
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 x-y,+x,+z+1/2
3 -y,x-y,+z
4 -x,-y,+z+1/2
5 y-x,-x,+z
6 +y,y-x,+z+1/2
-1 -x,-y,-z
-2 y-x,-x,-z+1/2
-3 +y,y-x,-z
-4 +x,+y,-z+1/2
-5 x-y,+x,-z
-6 -y,x-y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
La La1 0.23050(9) -0.01087(11) 0.25 1.0 Uani 0.0055 6
La La2 0.3333 0.6667 0.00077(17) 0.6625 Uani 0.01027 4
Ge Ge 0.40073(9) 0.37261(8) 0.25 1.0 Uani 0.00385 6
O O1 0.31200(16) 0.48703(17) 0.25 1.0 Uani 0.01152 6
O O2 0.60420(13) 0.47654(14) 0.25 1.0 Uani 0.01179 6
O O3 0.34181(15) 0.24837(12) 0.06139(12) 1.0 Uani 0.01955 12
O O4 0.0 0.0 0.25 0.873(10) Uani 0.01113 2
Sr Sr2 0.3333 0.6667 0.00077(17) 0.3375 Uani 0.01027 4
O O5 0.0197(24) 0.2543(19) 0.6044(19) 0.0490(25) Uiso 0.01 12
loop_
_atom_type_symbol
_atom_type_number_in_cell
La 8.65
Ge 6.0
O 26.334
Sr 1.35
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 La1 O2 98.17(5) 5_555 . 3_655 n
O1 La1 O3 145.052(30) 5_555 . 1_555 n
O1 La1 O3 69.39(4) 5_555 . 6_555 n
O1 La1 O3 69.39(4) 5_555 . -3_555 n
O1 La1 O3 145.052(30) 5_555 . -4_556 n
O1 La1 O4 112.32(4) 5_555 . 1_555 n
O1 La1 O5 55.1(4) 5_555 . 4_554 n
O1 La1 O5 87.8(4) 5_555 . 5_555 n
O1 La1 O5 154.86(34) 5_555 . 6_554 n
O1 La1 O5 55.1(4) 5_555 . -1_556 n
O1 La1 O5 87.8(4) 5_555 . -2_556 n
O1 La1 O5 154.86(34) 5_555 . -3_556 n
O2 La1 O3 70.15(4) 3_655 . 1_555 n
O2 La1 O3 85.766(32) 3_655 . 6_555 n
O2 La1 O3 85.766(32) 3_655 . -3_555 n
O2 La1 O3 70.15(4) 3_655 . -4_556 n
O2 La1 O4 149.51(6) 3_655 . 1_555 n
O2 La1 O5 142.2(4) 3_655 . 4_554 n
O2 La1 O5 89.2(4) 3_655 . 5_555 n
O2 La1 O5 87.1(4) 3_655 . 6_554 n
O2 La1 O5 142.2(4) 3_655 . -1_556 n
O2 La1 O5 89.2(4) 3_655 . -2_556 n
O2 La1 O5 87.1(4) 3_655 . -3_556 n
O3 La1 O3 138.49(5) 1_555 . 6_555 n
O3 La1 O3 76.813(21) 1_555 . -3_555 n
O3 La1 O3 63.56(4) 1_555 . -4_556 n
O3 La1 O4 84.10(4) 1_555 . 1_555 n
O3 La1 O5 114.80(31) 1_555 . 4_554 n
O3 La1 O5 123.6(5) 1_555 . 5_555 n
O3 La1 O5 19.2(4) 1_555 . 6_554 n
O3 La1 O5 147.2(4) 1_555 . -1_556 n
O3 La1 O5 60.1(5) 1_555 . -2_556 n
O3 La1 O5 59.70(33) 1_555 . -3_556 n
O3 La1 O3 136.12(8) 6_555 . -3_555 n
O3 La1 O3 76.813(21) 6_555 . -4_556 n
O3 La1 O4 104.446(34) 6_555 . 1_555 n
O3 La1 O5 105.03(30) 6_555 . 4_554 n
O3 La1 O5 19.5(4) 6_555 . 5_555 n
O3 La1 O5 135.7(4) 6_555 . 6_554 n
O3 La1 O5 61.15(33) 6_555 . -1_556 n
O3 La1 O5 155.6(4) 6_555 . -2_556 n
O3 La1 O5 86.6(4) 6_555 . -3_556 n
O3 La1 O3 138.49(5) -3_555 . -4_556 n
O3 La1 O4 104.446(34) -3_555 . 1_555 n
O3 La1 O5 61.15(33) -3_555 . 4_554 n
O3 La1 O5 155.6(4) -3_555 . 5_555 n
O3 La1 O5 86.6(4) -3_555 . 6_554 n
O3 La1 O5 105.03(30) -3_555 . -1_556 n
O3 La1 O5 19.5(4) -3_555 . -2_556 n
O3 La1 O5 135.7(4) -3_555 . -3_556 n
O3 La1 O4 84.10(4) -4_556 . 1_555 n
O3 La1 O5 147.2(4) -4_556 . 4_554 n
O3 La1 O5 60.1(5) -4_556 . 5_555 n
O3 La1 O5 59.70(33) -4_556 . 6_554 n
O3 La1 O5 114.80(31) -4_556 . -1_556 n
O3 La1 O5 123.6(5) -4_556 . -2_556 n
O3 La1 O5 19.2(4) -4_556 . -3_556 n
O4 La1 O5 63.5(4) 1_555 . 4_554 n
O4 La1 O5 91.9(4) 1_555 . 5_555 n
O4 La1 O5 65.4(4) 1_555 . 6_554 n
O4 La1 O5 63.5(4) 1_555 . -1_556 n
O4 La1 O5 91.9(4) 1_555 . -2_556 n
O4 La1 O5 65.4(4) 1_555 . -3_556 n
O5 La1 O5 113.1(6) 4_554 . 5_555 n
O5 La1 O5 107.1(6) 4_554 . 6_554 n
O5 La1 O5 47.1(6) 4_554 . -1_556 n
O5 La1 O5 66.0(5) 4_554 . -2_556 n
O5 La1 O5 128.9(6) 4_554 . -3_556 n
O5 La1 O5 117.0(7) 5_555 . 6_554 n
O5 La1 O5 66.0(5) 5_555 . -1_556 n
O5 La1 O5 175.0(8) 5_555 . -2_556 n
O5 La1 O5 67.6(4) 5_555 . -3_556 n
O5 La1 O5 128.9(6) 6_554 . -1_556 n
O5 La1 O5 67.6(4) 6_554 . -2_556 n
O5 La1 O5 49.4(7) 6_554 . -3_556 n
O5 La1 O5 113.1(6) -1_556 . -2_556 n
O5 La1 O5 107.1(6) -1_556 . -3_556 n
O5 La1 O5 117.0(7) -2_556 . -3_556 n
La2 La2 La2 179.9604 -2_564 . -2_565 n
La2 La2 O1 137.317(30) -2_565 . 1_555 n
La2 La2 O1 137.321(30) -2_565 . 3_665 n
La2 La2 O1 137.355(30) -2_565 . 5_565 n
La2 La2 O2 44.556(30) -2_565 . 2_554 n
La2 La2 O2 44.545(30) -2_565 . 4_664 n
La2 La2 O2 44.541(30) -2_565 . 6_564 n
La2 La2 Sr2 0.0 -2_565 . -2_565 n
La2 La2 Sr2 179.9604 -2_565 . -2_566 n
La2 La2 O1 42.671(30) -2_566 . 1_555 n
La2 La2 O1 42.661(30) -2_566 . 3_665 n
La2 La2 O1 42.676(30) -2_566 . 5_565 n
La2 La2 O2 135.474(30) -2_566 . 2_554 n
La2 La2 O2 135.432(30) -2_566 . 4_664 n
La2 La2 O2 135.452(30) -2_566 . 6_564 n
La2 La2 Sr2 179.9604 -2_566 . -2_565 n
La2 La2 Sr2 0.0 -2_566 . -2_566 n
O1 La2 O1 71.88(5) 1_555 . 3_665 n
O1 La2 O1 71.88(5) 1_555 . 5_565 n
O1 La2 O2 125.31(4) 1_555 . 2_554 n
O1 La2 O2 95.025(29) 1_555 . 4_664 n
O1 La2 O2 154.95(4) 1_555 . 6_564 n
O1 La2 Sr2 137.317(30) 1_555 . -2_565 n
O1 La2 Sr2 42.671(30) 1_555 . -2_566 n
O1 La2 O1 71.89(5) 3_665 . 5_565 n
O1 La2 O2 154.99(4) 3_665 . 2_554 n
O1 La2 O2 125.30(4) 3_665 . 4_664 n
O1 La2 O2 95.045(29) 3_665 . 6_564 n
O1 La2 Sr2 137.321(30) 3_665 . -2_565 n
O1 La2 Sr2 42.661(30) 3_665 . -2_566 n
O1 La2 O2 95.058(29) 5_565 . 2_554 n
O1 La2 O2 154.96(4) 5_565 . 4_664 n
O1 La2 O2 125.34(4) 5_565 . 6_564 n
O1 La2 Sr2 137.355(30) 5_565 . -2_565 n
O1 La2 Sr2 42.676(30) 5_565 . -2_566 n
O2 La2 O2 74.82(5) 2_554 . 4_664 n
O2 La2 O2 74.83(5) 2_554 . 6_564 n
O2 La2 Sr2 44.556(30) 2_554 . -2_565 n
O2 La2 Sr2 135.474(30) 2_554 . -2_566 n
O2 La2 O2 74.82(5) 4_664 . 6_564 n
O2 La2 Sr2 44.545(30) 4_664 . -2_565 n
O2 La2 Sr2 135.432(30) 4_664 . -2_566 n
O2 La2 Sr2 44.541(30) 6_564 . -2_565 n
O2 La2 Sr2 135.452(30) 6_564 . -2_566 n
Sr2 La2 Sr2 179.9604 -2_565 . -2_566 n
O1 Ge O2 115.11(8) 1_555 . 1_555 n
O1 Ge O3 110.98(5) 1_555 . 1_555 n
O1 Ge O3 110.98(5) 1_555 . -4_556 n
O1 Ge Sr2 138.26(4) 1_555 . 2_655 n
O1 Ge Sr2 138.26(4) 1_555 . -1_665 n
O1 Ge O5 91.0(7) 1_555 . 6_554 n
O1 Ge O5 91.0(7) 1_555 . -3_556 n
O2 Ge O3 107.23(6) 1_555 . 1_555 n
O2 Ge O3 107.23(6) 1_555 . -4_556 n
O2 Ge Sr2 48.200(35) 1_555 . 2_655 n
O2 Ge Sr2 48.193(35) 1_555 . -1_665 n
O2 Ge O5 135.6(6) 1_555 . 6_554 n
O2 Ge O5 135.6(6) 1_555 . -3_556 n
O3 Ge O3 104.71(8) 1_555 . -4_556 n
O3 Ge Sr2 110.70(5) 1_555 . 2_655 n
O3 Ge Sr2 59.66(5) 1_555 . -1_665 n
O3 Ge O5 28.5(6) 1_555 . 6_554 n
O3 Ge O5 94.4(5) 1_555 . -3_556 n
O3 Ge Sr2 59.66(5) -4_556 . 2_655 n
O3 Ge Sr2 110.69(5) -4_556 . -1_665 n
O3 Ge O5 94.4(5) -4_556 . 6_554 n
O3 Ge O5 28.5(6) -4_556 . -3_556 n
Sr2 Ge Sr2 65.65(4) 2_655 . -1_665 n
Sr2 Ge O5 128.5(7) 2_655 . 6_554 n
Sr2 Ge O5 88.2(6) 2_655 . -3_556 n
Sr2 Ge O5 88.2(6) -1_665 . 6_554 n
Sr2 Ge O5 128.5(7) -1_665 . -3_556 n
O5 Ge O5 74.2(10) 6_554 . -3_556 n
La1 O1 La2 107.46(4) 3_555 . 1_555 n
La1 O1 La2 107.47(4) 3_555 . -2_565 n
La1 O1 Ge 95.79(6) 3_555 . 1_555 n
La1 O1 Sr2 107.46(4) 3_555 . 1_555 n
La1 O1 Sr2 107.47(4) 3_555 . -2_566 n
La2 O1 La2 94.65(6) 1_555 . -2_565 n
La2 O1 Ge 125.07(4) 1_555 . 1_555 n
La2 O1 Sr2 0.0 1_555 . 1_555 n
La2 O1 Sr2 94.65(6) 1_555 . -2_566 n
La2 O1 Ge 125.05(4) -2_565 . 1_555 n
La2 O1 Sr2 94.65(6) -2_566 . 1_555 n
La2 O1 Sr2 0.0 -2_566 . -2_566 n
Ge O1 Sr2 125.07(4) 1_555 . 1_555 n
Ge O1 Sr2 125.05(4) 1_555 . -2_566 n
Sr2 O1 Sr2 94.65(6) 1_555 . -2_566 n
La1 O2 La2 117.40(4) 5_665 . 2_655 n
La1 O2 La2 117.39(4) 5_665 . -1_665 n
La1 O2 Ge 122.51(8) 5_665 . 1_555 n
La1 O2 Sr2 117.40(4) 5_665 . 2_655 n
La1 O2 Sr2 117.39(4) 5_665 . -1_665 n
La2 O2 La2 90.90(6) 2_655 . -1_665 n
La2 O2 Ge 101.49(4) 2_655 . 1_555 n
La2 O2 Sr2 0.0 2_655 . 2_655 n
La2 O2 Sr2 90.90(6) 2_655 . -1_665 n
La2 O2 Ge 101.51(4) -1_665 . 1_555 n
La2 O2 Sr2 90.90(6) -1_665 . 2_655 n
La2 O2 Sr2 0.0 -1_665 . -1_665 n
Ge O2 Sr2 101.49(4) 1_555 . 2_655 n
Ge O2 Sr2 101.51(4) 1_555 . -1_665 n
Sr2 O2 Sr2 90.90(6) 2_655 . -1_665 n
La1 O3 La1 117.46(5) 1_555 . 2_554 n
La1 O3 Ge 95.83(5) 1_555 . 1_555 n
La1 O3 Sr2 103.11(4) 1_555 . -1_665 n
La1 O3 O5 75.9(13) 1_555 . 6_554 n
La1 O3 Ge 139.98(6) 2_554 . 1_555 n
La1 O3 Sr2 102.90(5) 2_554 . -1_665 n
La1 O3 O5 89.4(9) 2_554 . 6_554 n
Ge O3 Sr2 89.35(6) 1_555 . -1_665 n
Ge O3 O5 77.2(10) 1_555 . 6_554 n
Sr2 O3 O5 166.3(10) -1_665 . 6_554 n
La1 O4 La1 120.0 1_555 . 3_555 n
La1 O4 La1 120.0 1_555 . 5_555 n
La1 O4 La1 120.0 3_555 . 5_555 n
La2 Sr2 La2 179.9604 -2_564 . -2_565 n
La2 Sr2 Ge 57.181(19) -2_564 . 2_554 n
La2 Sr2 Ge 57.162(19) -2_564 . 4_664 n
La2 Sr2 Ge 57.174(19) -2_564 . 6_564 n
La2 Sr2 O1 137.317(30) -2_565 . 1_555 n
La2 Sr2 O1 137.321(30) -2_565 . 3_665 n
La2 Sr2 O1 137.355(30) -2_565 . 5_565 n
La2 Sr2 O2 44.556(30) -2_565 . 2_554 n
La2 Sr2 O2 44.545(30) -2_565 . 4_664 n
La2 Sr2 O2 44.541(30) -2_565 . 6_564 n
La2 Sr2 O3 81.030(29) -2_565 . -1_665 n
La2 Sr2 O3 81.052(29) -2_565 . -3_565 n
La2 Sr2 O3 81.048(29) -2_565 . -5_555 n
La2 Sr2 Sr2 0.0 -2_565 . -2_565 n
La2 Sr2 Sr2 179.9604 -2_565 . -2_566 n
La2 Sr2 Ge 122.838(19) -2_565 . 2_554 n
La2 Sr2 Ge 122.807(19) -2_565 . 4_664 n
La2 Sr2 Ge 122.838(19) -2_565 . 6_564 n
La2 Sr2 O1 42.671(30) -2_566 . 1_555 n
La2 Sr2 O1 42.661(30) -2_566 . 3_665 n
La2 Sr2 O1 42.676(30) -2_566 . 5_565 n
La2 Sr2 O2 135.474(30) -2_566 . 2_554 n
La2 Sr2 O2 135.432(30) -2_566 . 4_664 n
La2 Sr2 O2 135.452(30) -2_566 . 6_564 n
La2 Sr2 O3 98.940(29) -2_566 . -1_665 n
La2 Sr2 O3 98.969(29) -2_566 . -3_565 n
La2 Sr2 O3 98.960(29) -2_566 . -5_555 n
La2 Sr2 Sr2 179.9604 -2_566 . -2_565 n
La2 Sr2 Sr2 0.0 -2_566 . -2_566 n
Ge Sr2 Ge 93.385(25) 2_554 . 4_664 n
Ge Sr2 Ge 93.400(25) 2_554 . 6_564 n
Ge Sr2 O1 96.807(33) 2_554 . 1_555 n
Ge Sr2 O1 165.49(4) 2_554 . 3_665 n
Ge Sr2 O1 96.272(22) 2_554 . 5_565 n
Ge Sr2 O2 30.302(26) 2_554 . 2_554 n
Ge Sr2 O2 63.399(31) 2_554 . 4_664 n
Ge Sr2 O2 98.75(4) 2_554 . 6_564 n
Ge Sr2 O3 124.34(4) 2_554 . -1_665 n
Ge Sr2 O3 92.290(29) 2_554 . -3_565 n
Ge Sr2 O3 30.992(21) 2_554 . -5_555 n
Ge Sr2 Sr2 57.181(19) 2_554 . -2_565 n
Ge Sr2 Sr2 122.838(19) 2_554 . -2_566 n
Ge Sr2 Ge 93.391(25) 4_664 . 6_564 n
Ge Sr2 O1 96.246(22) 4_664 . 1_555 n
Ge Sr2 O1 96.800(33) 4_664 . 3_665 n
Ge Sr2 O1 165.48(4) 4_664 . 5_565 n
Ge Sr2 O2 98.74(4) 4_664 . 2_554 n
Ge Sr2 O2 30.297(26) 4_664 . 4_664 n
Ge Sr2 O2 63.395(31) 4_664 . 6_564 n
Ge Sr2 O3 30.987(21) 4_664 . -1_665 n
Ge Sr2 O3 124.36(4) 4_664 . -3_565 n
Ge Sr2 O3 92.268(29) 4_664 . -5_555 n
Ge Sr2 Sr2 57.162(19) 4_664 . -2_565 n
Ge Sr2 Sr2 122.807(19) 4_664 . -2_566 n
Ge Sr2 O1 165.50(4) 6_564 . 1_555 n
Ge Sr2 O1 96.272(22) 6_564 . 3_665 n
Ge Sr2 O1 96.829(33) 6_564 . 5_565 n
Ge Sr2 O2 63.410(31) 6_564 . 2_554 n
Ge Sr2 O2 98.75(4) 6_564 . 4_664 n
Ge Sr2 O2 30.307(26) 6_564 . 6_564 n
Ge Sr2 O3 92.280(29) 6_564 . -1_665 n
Ge Sr2 O3 30.995(21) 6_564 . -3_565 n
Ge Sr2 O3 124.36(4) 6_564 . -5_555 n
Ge Sr2 Sr2 57.174(19) 6_564 . -2_565 n
Ge Sr2 Sr2 122.838(19) 6_564 . -2_566 n
O1 Sr2 O1 71.88(5) 1_555 . 3_665 n
O1 Sr2 O1 71.88(5) 1_555 . 5_565 n
O1 Sr2 O2 125.31(4) 1_555 . 2_554 n
O1 Sr2 O2 95.025(29) 1_555 . 4_664 n
O1 Sr2 O2 154.95(4) 1_555 . 6_564 n
O1 Sr2 O3 90.44(4) 1_555 . -1_665 n
O1 Sr2 O3 137.76(5) 1_555 . -3_565 n
O1 Sr2 O3 66.12(4) 1_555 . -5_555 n
O1 Sr2 Sr2 137.317(30) 1_555 . -2_565 n
O1 Sr2 Sr2 42.671(30) 1_555 . -2_566 n
O1 Sr2 O1 71.89(5) 3_665 . 5_565 n
O1 Sr2 O2 154.99(4) 3_665 . 2_554 n
O1 Sr2 O2 125.30(4) 3_665 . 4_664 n
O1 Sr2 O2 95.045(29) 3_665 . 6_564 n
O1 Sr2 O3 66.12(4) 3_665 . -1_665 n
O1 Sr2 O3 90.47(4) 3_665 . -3_565 n
O1 Sr2 O3 137.73(5) 3_665 . -5_555 n
O1 Sr2 Sr2 137.321(30) 3_665 . -2_565 n
O1 Sr2 Sr2 42.661(30) 3_665 . -2_566 n
O1 Sr2 O2 95.058(29) 5_565 . 2_554 n
O1 Sr2 O2 154.96(4) 5_565 . 4_664 n
O1 Sr2 O2 125.34(4) 5_565 . 6_564 n
O1 Sr2 O3 137.74(5) 5_565 . -1_665 n
O1 Sr2 O3 66.14(4) 5_565 . -3_565 n
O1 Sr2 O3 90.46(4) 5_565 . -5_555 n
O1 Sr2 Sr2 137.355(30) 5_565 . -2_565 n
O1 Sr2 Sr2 42.676(30) 5_565 . -2_566 n
O2 Sr2 O2 74.82(5) 2_554 . 4_664 n
O2 Sr2 O2 74.83(5) 2_554 . 6_564 n
O2 Sr2 O3 125.53(5) 2_554 . -1_665 n
O2 Sr2 O3 64.571(34) 2_554 . -3_565 n
O2 Sr2 O3 61.018(29) 2_554 . -5_555 n
O2 Sr2 Sr2 44.556(30) 2_554 . -2_565 n
O2 Sr2 Sr2 135.474(30) 2_554 . -2_566 n
O2 Sr2 O2 74.82(5) 4_664 . 6_564 n
O2 Sr2 O3 61.007(29) 4_664 . -1_665 n
O2 Sr2 O3 125.55(5) 4_664 . -3_565 n
O2 Sr2 O3 64.553(34) 4_664 . -5_555 n
O2 Sr2 Sr2 44.545(30) 4_664 . -2_565 n
O2 Sr2 Sr2 135.432(30) 4_664 . -2_566 n
O2 Sr2 O3 64.555(34) 6_564 . -1_665 n
O2 Sr2 O3 61.026(29) 6_564 . -3_565 n
O2 Sr2 O3 125.54(5) 6_564 . -5_555 n
O2 Sr2 Sr2 44.541(30) 6_564 . -2_565 n
O2 Sr2 Sr2 135.452(30) 6_564 . -2_566 n
O3 Sr2 O3 117.627(15) -1_665 . -3_565 n
O3 Sr2 O3 117.605(15) -1_665 . -5_555 n
O3 Sr2 Sr2 81.030(29) -1_665 . -2_565 n
O3 Sr2 Sr2 98.940(29) -1_665 . -2_566 n
O3 Sr2 O3 117.635(15) -3_565 . -5_555 n
O3 Sr2 Sr2 81.052(29) -3_565 . -2_565 n
O3 Sr2 Sr2 98.969(29) -3_565 . -2_566 n
O3 Sr2 Sr2 81.048(29) -5_555 . -2_565 n
O3 Sr2 Sr2 98.960(29) -5_555 . -2_566 n
Sr2 Sr2 Sr2 179.9604 -2_565 . -2_566 n
La1 O5 La1 115.0(7) 2_555 . 3_555 n
La1 O5 La1 101.7(6) 2_555 . 4_555 n
La1 O5 Ge 97.7(7) 2_555 . 2_555 n
La1 O5 O3 84.9(14) 2_555 . 2_555 n
La1 O5 La1 111.2(6) 3_555 . 4_555 n
La1 O5 Ge 129.0(8) 3_555 . 2_555 n
La1 O5 O3 71.1(9) 3_555 . 2_555 n
La1 O5 Ge 98.1(8) 4_555 . 2_555 n
La1 O5 O3 170.6(16) 4_555 . 2_555 n
Ge O5 O3 74.2(10) 2_555 . 2_555 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 La1 4.0453(14) . 3_555 n
La1 La1 4.0453(14) . 5_555 n
La1 Ge 3.2919(12) . 1_555 n
La1 Ge 3.3984(13) . 5_555 n
La1 O1 2.7457(18) . 5_555 n
La1 O2 2.5108(14) . 3_655 n
La1 O3 2.6210(14) . 1_555 n
La1 O3 2.4568(9) . 6_555 n
La1 O3 2.4568(9) . -3_555 n
La1 O3 2.6210(14) . -4_555 n
La1 O4 2.3356(8) . 1_555 n
La1 Sr2 4.2161(10) . 1_545 n
La1 Sr2 4.3451(10) . 2_655 n
La1 Sr2 4.3457(10) . -1_665 n
La1 Sr2 4.2167(10) . -2_555 n
La1 O5 2.664(19) . 4_554 n
La1 O5 2.596(14) . 5_555 n
La1 O5 2.552(19) . 6_554 n
La1 O5 2.664(19) . -1_556 n
La1 O5 2.596(14) . -2_555 n
La1 O5 2.552(19) . -3_556 n
La2 La2 3.6705(25) . -2_564 n
La2 La2 3.6479(25) . -2_565 n
La2 Ge 3.3853(10) . 2_554 n
La2 Ge 3.3858(10) . 4_664 n
La2 Ge 3.3850(10) . 6_564 n
La2 O1 2.4809(12) . 1_555 n
La2 O1 2.4806(12) . 3_665 n
La2 O1 2.4802(12) . 5_565 n
La2 O2 2.5749(13) . 2_554 n
La2 O2 2.5756(13) . 4_664 n
La2 O2 2.5751(13) . 6_564 n
La2 O3 2.9224(14) . -1_665 n
La2 O3 2.9215(14) . -3_565 n
La2 O3 2.9222(14) . -5_555 n
La2 Sr2 3.6705(25) . -2_564 n
La2 Sr2 3.6479(25) . -2_565 n
Ge La1 3.2919(12) . 1_555 n
Ge La1 3.3984(13) . 3_555 n
Ge La2 3.3850(10) . 2_655 n
Ge La2 3.3858(10) . -1_665 n
Ge O1 1.7448(11) . 1_555 n
Ge O2 1.7431(14) . 1_555 n
Ge O3 1.7433(9) . 1_555 n
Ge O3 1.7433(9) . -4_555 n
Ge Sr2 3.7648(9) . 1_555 n
Ge Sr2 3.3850(10) . 2_655 n
Ge Sr2 3.3858(10) . -1_665 n
Ge Sr2 3.7642(9) . -2_565 n
Ge O5 1.767(15) . 6_554 n
Ge O5 1.767(15) . -3_556 n
O1 La1 2.7457(18) . 3_555 n
O1 La2 2.4809(12) . 1_555 n
O1 La2 2.4806(12) . -2_565 n
O1 Ge 1.7448(11) . 1_555 n
O1 Sr2 2.4809(12) . 1_555 n
O1 Sr2 2.4806(12) . -2_565 n
O2 La1 2.5108(14) . 5_665 n
O2 La2 2.5751(13) . 2_655 n
O2 La2 2.5756(13) . -1_665 n
O2 Ge 1.7431(14) . 1_555 n
O2 Sr2 2.5751(13) . 2_655 n
O2 Sr2 2.5756(13) . -1_665 n
O3 La1 2.6210(14) . 1_555 n
O3 La1 2.4568(9) . 2_554 n
O3 La2 2.9224(14) . -1_665 n
O3 Ge 1.7433(9) . 1_555 n
O3 Sr2 2.9224(14) . -1_665 n
O3 O5 0.866(18) . 6_554 n
O4 La1 2.3356(8) . 1_555 n
O4 La1 2.3356(8) . 3_555 n
O4 La1 2.3356(8) . 5_555 n
Sr2 La1 4.2161(10) . 1_565 n
Sr2 La1 4.3460(10) . 2_554 n
Sr2 La1 4.2167(10) . 3_555 n
Sr2 La1 4.3457(10) . 4_664 n
Sr2 La1 4.2169(10) . 5_665 n
Sr2 La1 4.3451(10) . 6_564 n
Sr2 La2 3.6705(25) . -2_564 n
Sr2 La2 3.6479(25) . -2_565 n
Sr2 Ge 3.7648(9) . 1_555 n
Sr2 Ge 3.3853(10) . 2_554 n
Sr2 Ge 3.7642(9) . 3_665 n
Sr2 Ge 3.3858(10) . 4_664 n
Sr2 Ge 3.7639(9) . 5_565 n
Sr2 Ge 3.3850(10) . 6_564 n
Sr2 O1 2.4809(12) . 1_555 n
Sr2 O1 2.4806(12) . 3_665 n
Sr2 O1 2.4802(12) . 5_565 n
Sr2 O2 2.5749(13) . 2_554 n
Sr2 O2 2.5756(13) . 4_664 n
Sr2 O2 2.5751(13) . 6_564 n
Sr2 O3 2.9224(14) . -1_665 n
Sr2 O3 2.9215(14) . -3_565 n
Sr2 O3 2.9222(14) . -5_555 n
Sr2 Sr2 3.6705(25) . -2_564 n
Sr2 Sr2 3.6479(25) . -2_565 n
O5 La1 2.552(19) . 2_555 n
O5 La1 2.596(14) . 3_555 n
O5 La1 2.664(19) . 4_555 n
O5 Ge 1.767(15) . 2_555 n
O5 O3 0.866(18) . 2_555 n
O5 O5 2.131(29) . -4_556 n
